NANOSYSTEMS: PHYSICS, CHEMISTRY, MATHEMATICS, 2016, 7 (6), P. 919–924

Macroscopic thermoelectric efficiency of carbon nanocomposites E. D. Eidelman1,2 , A. P. Meilakhs1 1

1Ioffe Physical Technical Institute, 26 Politekhnicheskaya, 194021 Saint Petersburg, Russia 2

Saint Petersburg State Chemical-Pharmaceutical Academy, 14 Professora Popova, 197376 Saint Petersburg, Russia [email protected], [email protected]

PACS 84.60.Rb, 85.80.Fi

DOI 10.17586/2220-8054-2016-7-6-919-924

The subject of this study is the thermoelectric efficiency (Z) and the thermoelectric parameter (ZT ) of carbon nanocomposites, namely, the structures consisting of graphite-like (gr) and diamond-like (d) regions made of sp2 and sp3 hybridized carbon atoms, respectively. The impact of heat transfer across the boundary between sp2 and sp3 areas is analyzed for the first time. It is shown that the interfacial thermal resistance (Kapitza resistance) is not lower than the thermal resistance in the macroscopic gr region. The influence of various factors on the Kapitza resistance is analyzed. The value of ZT ≈ 3.5 at room temperature, taking into account the interfacial thermal resistance, is significantly higher than it would be in gr films (ZT ≈ 0.75). Keywords: carbon nanostructures, thermoelectricity. Received: 28 October 2016

1.

Introduction

In recent years, a lot of attention has been paid to the influence of size on transport phenomena in solids and, in particular, on thermoelectric effects [1–5]. Currently, attention is focused on the creation of new materials with the highest possible thermoelectric figure of merit (quality factor) Z, which makes it possible to use this material in refrigerators or generators [2,5]: Z = S 2 σ/χ. Here, S is the thermoelectric coefficient or the Seebeck coefficient (V/K), σ is the conductivity ratio ((Ohm·m) -1), and χ is the thermal conductivity (J/(m·s·K)). The higher the value of the parameter ZT (where T is the temperature in Kelvin) is for any material, the more useful this material is for thermoelectric conversion. Therefore, ZT is used as a dimensionless quantity that characterizes thermoelectric materials. Serious efforts were made to increase Z, both by selecting an appropriate semiconductor and by determining its optimal layer thickness [3, 4]. To the best of the authors’ knowledge, the highest value ZT = 2.6 at room temperature is reported in [6] for SnSe crystals. Part of this effort is the study of thermoelectric phenomena in carbon nanostructures [3–5]. In these nanostructures, hybridized carbon atoms coexist. The coexistence of regions with very different electrical and thermal properties at such small distances from each other is a unique feature of these structures. The gr areas are semimetallic with a high electrical conductivity but a relatively low thermal conductivity. The d areas are wide bandgap semiconductors, dielectrics in fact, but with a high thermal conductivity. The corresponding kinetic coefficients differ in value by many orders of magnitude. The article deals with the Z values of the composite produced from 4 nm diamond nanoparticles generated by detonation synthesis. Such diamond nanoparticles were prepared by milling [7–9] and before long by purification techniques [10, 11] from agglomerates about 100 nm in size. Then, solid composite was produced from 4 nm particles by sintering at high pressure and high temperature (HPHT). Regions with sp3 hybridization, as determined by areas of coherence, reached sizes of up to 4-12 nm. The composite consists of such particles with a d core, which can be covered by up to four layers of the sp2 phase, but may have no coating at all. The composite is completely free from the separate gr phase. The average particle size becomes 4-35 nm [12]. Then, the size of gr regions can be assumed at an average of l ≈ 10–30 nm. The thermoelectric effect and mechanisms that contribute to the increase in the thermoelectric coefficient S, the main component of the Z, were discussed in [13, 14] for carbon nanostructures. As for the ratio of electrical and thermal conductivity coefficients σ/χ being part of Z, it is always considered to be proportional to the temperature according to the Wiedemann - Franz law (see, e.g., [15] §78). Of course, there may be limitations associated with the possible flow of heat in the gr areas. Let us further assume that the percolation threshold (see, eg, [16]) is reached [9], but the heat carried by electrons is small compared with the lattice vibrations heat transfer.

920

E. D. Eidelman, A. P. Meilakhs

It was recently shown that the presence of borders between the gr and d regions greatly influences the thermal conductivity of carbon nanostructures [17,18]. In this paper, we examine the effect of borders on the thermoelectric efficiency. 2.

Statement of the problem of heat transfer through the interface between phases

Let us assume that the gr area is heated or cooled on one side and contacts with a d area on the other side. In this case, the gr phonons migrate into d or d phonons migrate into gr. In accordance with Fourier’s law, this heat source lowers or raises the temperature of the gr lattice. The heat of the electron gas from the gr area is not directly transferred to the d area. However, the electrons can heat or cool the crystal lattice in gr. An increase in the phonon flux component takes place, and then the heat is transferred from this component to the d area. This nonlinear process occurs due to the temperature difference between the electronic and phonon subsystems in gr. It appears as a result of presence of the boundary with d. The ideal structure would be the one with plane borders perpendicular to the direction of heat propagation. Any possibility of heat flow bypassing the border increases the thermal conductivity, and thus reduces the thermoelectric efficiency Z. The temperature at the border undergoes a jump ∆T , which is proportional to the heat flux q (W/m2 ). Such dependence makes it possible to use the electrothermal analogy. The proportionality coefficient r (m2 ·K/W) between the ∆T and q is called interfacial thermal resistance (Kapitza resistance). The Kapitza resistance is a characteristic of the interface; in the heat transfer theory the reciprocal value of 1/r is called the heat transfer coefficient. The process being considered is a special case of heat transfer through the metal – dielectric boundary. The Kapitza resistance at the metal-dielectric interface has been widely studied (see, e.g., [17]). It was found that the Kapitza resistance, as calculated considering the nonlinearity of the process, does not depend on the dielectric characteristics and is fully determined by the properties of the metal. This thesis was experimentally confirmed in [19]. In fact, each subsystem in gr is characterized by its set of values: electron Te ; qe : χe , and phonon Tph , qph , χph . Each triplet of values is related according to the Fourier law. The interaction coefficient θ (W/(m3 ·K)) characterizes the efficiency of heat transfer between subsystems and relates the heat flux to the difference Te − Tph . It should be noted that in experiments, the temperature is measured far away from the boundary. At this location, the temperature is Te = Tph = T , and the thermal conductivity χ = χe + χph can be attributable to the general heat flow in gr: q = qe + qph . In gr, it can be assumed that χe >> χph and heat transfer through the electronic subsystem dominates. Only phonons can pass from gr to d, hence qph = q; qe = 0 at the boundary. According to [19], the problem is posed so that the properties of d do not affect the Te and Tph temperature in gr. 3.

Temperature and thermal resistance alignment at the boundary between gr and d

The solution of the problem is completely similar to that provided in [17]. The result is that the characteristic distance λ, at which the temperatures of the electron and phonon subsystems in gr are actually aligned, is related to the system characteristics as: r χe χph 1/2 ' (χph /θ) . (1) λ= θχ The components of the thermal resistance are determined by the jumps of the subsystems temperatures, Te (0) and Tph (0), relative to the temperature Td in d, which is equal to Td (0) at the boundary (Fig. 1). In the course of the experiment, the temperature gradient from a region far from the boundary is usually extrapolated linearly to the boundary. This temperature Tgr is considered to be the gr temperature; accordingly, it is Tgr (0) at the border, and the temperature jump is considered equal to ∆T = Tgr (0) − Td (0). However, almost always Tgr (0) ≈ Te (0). The Kapitza thermal resistance caused by the measured jump ∆T can be divided into rph , arising due to the temperature jump ∆Tph of phonons in gr and d areas, and rr , arising because the electronic and phonon subsystems in gr are heated unequally near the border. Therefore, r = rph + rr . The thermal resistance (relative!) rr arises due to the difference in temperature jumps of the electron ∆Te and phonon ∆Tph subsystems: ∆Tr = Te − Tph = ∆Te − ∆Tph . In practice, the temperature in gr is determined by the electronic subsystem temperature. So, the measured jump ∆T ≈ ∆Te and ∆Tr can be calculated as ∆Tr = ∆T − ∆Tph .

Macroscopic thermoelectric efficiency of carbon nanocomposites

921

F IG . 1. This figure presents the temperatures in the graphite-like (gr) area Tgr (on the right) and the diamond-like (d) area Td (on the left), near the boundary located at x = 0. At the boundary, the temperatures are, respectively, Tgr (0), Td (0), Te (0) and Tph (0). Also shown are values of the corresponding temperature jumps ∆Tph and ∆Te at the border to the temperature T d (0). The jump ∆T = T gr(0) − T d (0) is measured experimentally. Finally, the temperature differences in gr subsystems were shown to be caused by the Kapitza resistance due to the presence of the boundary ∆Tr The value of the jump ∆Tph determines the proportion of phonons reflected from the boundary back into gr. This proportion was determined in [13] for a system very similar to the carbon nanocomposites under study. There, it was found to be usually small. Therefore, ∆Tph

Macroscopic thermoelectric efficiency of carbon nanocomposites E. D. Eidelman1,2 , A. P. Meilakhs1 1

1Ioffe Physical Technical Institute, 26 Politekhnicheskaya, 194021 Saint Petersburg, Russia 2

Saint Petersburg State Chemical-Pharmaceutical Academy, 14 Professora Popova, 197376 Saint Petersburg, Russia [email protected], [email protected]

PACS 84.60.Rb, 85.80.Fi

DOI 10.17586/2220-8054-2016-7-6-919-924

The subject of this study is the thermoelectric efficiency (Z) and the thermoelectric parameter (ZT ) of carbon nanocomposites, namely, the structures consisting of graphite-like (gr) and diamond-like (d) regions made of sp2 and sp3 hybridized carbon atoms, respectively. The impact of heat transfer across the boundary between sp2 and sp3 areas is analyzed for the first time. It is shown that the interfacial thermal resistance (Kapitza resistance) is not lower than the thermal resistance in the macroscopic gr region. The influence of various factors on the Kapitza resistance is analyzed. The value of ZT ≈ 3.5 at room temperature, taking into account the interfacial thermal resistance, is significantly higher than it would be in gr films (ZT ≈ 0.75). Keywords: carbon nanostructures, thermoelectricity. Received: 28 October 2016

1.

Introduction

In recent years, a lot of attention has been paid to the influence of size on transport phenomena in solids and, in particular, on thermoelectric effects [1–5]. Currently, attention is focused on the creation of new materials with the highest possible thermoelectric figure of merit (quality factor) Z, which makes it possible to use this material in refrigerators or generators [2,5]: Z = S 2 σ/χ. Here, S is the thermoelectric coefficient or the Seebeck coefficient (V/K), σ is the conductivity ratio ((Ohm·m) -1), and χ is the thermal conductivity (J/(m·s·K)). The higher the value of the parameter ZT (where T is the temperature in Kelvin) is for any material, the more useful this material is for thermoelectric conversion. Therefore, ZT is used as a dimensionless quantity that characterizes thermoelectric materials. Serious efforts were made to increase Z, both by selecting an appropriate semiconductor and by determining its optimal layer thickness [3, 4]. To the best of the authors’ knowledge, the highest value ZT = 2.6 at room temperature is reported in [6] for SnSe crystals. Part of this effort is the study of thermoelectric phenomena in carbon nanostructures [3–5]. In these nanostructures, hybridized carbon atoms coexist. The coexistence of regions with very different electrical and thermal properties at such small distances from each other is a unique feature of these structures. The gr areas are semimetallic with a high electrical conductivity but a relatively low thermal conductivity. The d areas are wide bandgap semiconductors, dielectrics in fact, but with a high thermal conductivity. The corresponding kinetic coefficients differ in value by many orders of magnitude. The article deals with the Z values of the composite produced from 4 nm diamond nanoparticles generated by detonation synthesis. Such diamond nanoparticles were prepared by milling [7–9] and before long by purification techniques [10, 11] from agglomerates about 100 nm in size. Then, solid composite was produced from 4 nm particles by sintering at high pressure and high temperature (HPHT). Regions with sp3 hybridization, as determined by areas of coherence, reached sizes of up to 4-12 nm. The composite consists of such particles with a d core, which can be covered by up to four layers of the sp2 phase, but may have no coating at all. The composite is completely free from the separate gr phase. The average particle size becomes 4-35 nm [12]. Then, the size of gr regions can be assumed at an average of l ≈ 10–30 nm. The thermoelectric effect and mechanisms that contribute to the increase in the thermoelectric coefficient S, the main component of the Z, were discussed in [13, 14] for carbon nanostructures. As for the ratio of electrical and thermal conductivity coefficients σ/χ being part of Z, it is always considered to be proportional to the temperature according to the Wiedemann - Franz law (see, e.g., [15] §78). Of course, there may be limitations associated with the possible flow of heat in the gr areas. Let us further assume that the percolation threshold (see, eg, [16]) is reached [9], but the heat carried by electrons is small compared with the lattice vibrations heat transfer.

920

E. D. Eidelman, A. P. Meilakhs

It was recently shown that the presence of borders between the gr and d regions greatly influences the thermal conductivity of carbon nanostructures [17,18]. In this paper, we examine the effect of borders on the thermoelectric efficiency. 2.

Statement of the problem of heat transfer through the interface between phases

Let us assume that the gr area is heated or cooled on one side and contacts with a d area on the other side. In this case, the gr phonons migrate into d or d phonons migrate into gr. In accordance with Fourier’s law, this heat source lowers or raises the temperature of the gr lattice. The heat of the electron gas from the gr area is not directly transferred to the d area. However, the electrons can heat or cool the crystal lattice in gr. An increase in the phonon flux component takes place, and then the heat is transferred from this component to the d area. This nonlinear process occurs due to the temperature difference between the electronic and phonon subsystems in gr. It appears as a result of presence of the boundary with d. The ideal structure would be the one with plane borders perpendicular to the direction of heat propagation. Any possibility of heat flow bypassing the border increases the thermal conductivity, and thus reduces the thermoelectric efficiency Z. The temperature at the border undergoes a jump ∆T , which is proportional to the heat flux q (W/m2 ). Such dependence makes it possible to use the electrothermal analogy. The proportionality coefficient r (m2 ·K/W) between the ∆T and q is called interfacial thermal resistance (Kapitza resistance). The Kapitza resistance is a characteristic of the interface; in the heat transfer theory the reciprocal value of 1/r is called the heat transfer coefficient. The process being considered is a special case of heat transfer through the metal – dielectric boundary. The Kapitza resistance at the metal-dielectric interface has been widely studied (see, e.g., [17]). It was found that the Kapitza resistance, as calculated considering the nonlinearity of the process, does not depend on the dielectric characteristics and is fully determined by the properties of the metal. This thesis was experimentally confirmed in [19]. In fact, each subsystem in gr is characterized by its set of values: electron Te ; qe : χe , and phonon Tph , qph , χph . Each triplet of values is related according to the Fourier law. The interaction coefficient θ (W/(m3 ·K)) characterizes the efficiency of heat transfer between subsystems and relates the heat flux to the difference Te − Tph . It should be noted that in experiments, the temperature is measured far away from the boundary. At this location, the temperature is Te = Tph = T , and the thermal conductivity χ = χe + χph can be attributable to the general heat flow in gr: q = qe + qph . In gr, it can be assumed that χe >> χph and heat transfer through the electronic subsystem dominates. Only phonons can pass from gr to d, hence qph = q; qe = 0 at the boundary. According to [19], the problem is posed so that the properties of d do not affect the Te and Tph temperature in gr. 3.

Temperature and thermal resistance alignment at the boundary between gr and d

The solution of the problem is completely similar to that provided in [17]. The result is that the characteristic distance λ, at which the temperatures of the electron and phonon subsystems in gr are actually aligned, is related to the system characteristics as: r χe χph 1/2 ' (χph /θ) . (1) λ= θχ The components of the thermal resistance are determined by the jumps of the subsystems temperatures, Te (0) and Tph (0), relative to the temperature Td in d, which is equal to Td (0) at the boundary (Fig. 1). In the course of the experiment, the temperature gradient from a region far from the boundary is usually extrapolated linearly to the boundary. This temperature Tgr is considered to be the gr temperature; accordingly, it is Tgr (0) at the border, and the temperature jump is considered equal to ∆T = Tgr (0) − Td (0). However, almost always Tgr (0) ≈ Te (0). The Kapitza thermal resistance caused by the measured jump ∆T can be divided into rph , arising due to the temperature jump ∆Tph of phonons in gr and d areas, and rr , arising because the electronic and phonon subsystems in gr are heated unequally near the border. Therefore, r = rph + rr . The thermal resistance (relative!) rr arises due to the difference in temperature jumps of the electron ∆Te and phonon ∆Tph subsystems: ∆Tr = Te − Tph = ∆Te − ∆Tph . In practice, the temperature in gr is determined by the electronic subsystem temperature. So, the measured jump ∆T ≈ ∆Te and ∆Tr can be calculated as ∆Tr = ∆T − ∆Tph .

Macroscopic thermoelectric efficiency of carbon nanocomposites

921

F IG . 1. This figure presents the temperatures in the graphite-like (gr) area Tgr (on the right) and the diamond-like (d) area Td (on the left), near the boundary located at x = 0. At the boundary, the temperatures are, respectively, Tgr (0), Td (0), Te (0) and Tph (0). Also shown are values of the corresponding temperature jumps ∆Tph and ∆Te at the border to the temperature T d (0). The jump ∆T = T gr(0) − T d (0) is measured experimentally. Finally, the temperature differences in gr subsystems were shown to be caused by the Kapitza resistance due to the presence of the boundary ∆Tr The value of the jump ∆Tph determines the proportion of phonons reflected from the boundary back into gr. This proportion was determined in [13] for a system very similar to the carbon nanocomposites under study. There, it was found to be usually small. Therefore, ∆Tph